#------------------------------------------------------------------------------
#$Date: 2020-08-22 02:04:26 +0300 (Sat, 22 Aug 2020) $
#$Revision: 255552 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/13/51/4135199.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4135199
loop_
_publ_author_name
'Yan, Yong'
'Carrington, Elliot J.'
'Pétuya, Rémi'
'Whitehead, George F. S.'
'Verma, Ajay'
'Hylton, Rebecca K.'
'Tang, Chiu C.'
'Berry, Neil G.'
'Darling, George R.'
'Dyer, Matthew S.'
'Antypov, Dmytro'
'Katsoulidis, Alexandros P.'
'Rosseinsky, Matthew J.'
_publ_section_title
;
 Amino Acid Residues Determine the Response of Flexible Metal-Organic
 Frameworks to Guests.
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_paper_doi               10.1021/jacs.0c03853
_journal_year                    2020
_chemical_formula_moiety         'C6 H5 N3 O3 Zn, 0.84(C1 H2 Cl2)'
_chemical_formula_sum            'C6.84 H6.68 Cl1.68 N3 O3 Zn'
_chemical_formula_weight         303.98
_space_group_crystal_system      trigonal
_space_group_IT_number           161
_space_group_name_Hall           'R 3 -2"c'
_space_group_name_H-M_alt        'R 3 c :H'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_audit_creation_date             2018-07-05
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            18
_cell_length_a                   27.1513(6)
_cell_length_b                   27.1513(6)
_cell_length_c                   10.1334(2)
_cell_measurement_reflns_used    14377
_cell_measurement_temperature    100
_cell_measurement_theta_max      27.4450
_cell_measurement_theta_min      2.5880
_cell_volume                     6469.4(2)
_computing_cell_refinement       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'XS (Sheldrick, 2008)'
_diffrn_ambient_temperature      100
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
--------------------------------------------------------------------------
  1  ω   -110.00  15.00   1.00   10.00    --  -20.00 -68.00   0.00  125
  2  ω   -110.00  15.00   1.00   10.00    --  -20.00 -68.00 120.00  125
  3  ω   -110.00  15.00   1.00   10.00    --  -20.00 -68.00 240.00  125
  4  ω   -110.00  15.00   1.00   10.00    --  -20.00 -30.00  90.00  125
;
_diffrn_measurement_device       'abstract diffractometer'
_diffrn_measurement_device_type
'Rigaku Rotating Anode Diffractometer withb Saturn Detector'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0093144000
_diffrn_orient_matrix_UB_12      -0.0200400000
_diffrn_orient_matrix_UB_13      -0.0076987000
_diffrn_orient_matrix_UB_21      0.0284871000
_diffrn_orient_matrix_UB_22      0.0218614000
_diffrn_orient_matrix_UB_23      0.0105179000
_diffrn_orient_matrix_UB_31      -0.0033068000
_diffrn_orient_matrix_UB_32      -0.0055864000
_diffrn_orient_matrix_UB_33      0.0687475000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0479
_diffrn_reflns_av_unetI/netI     0.0233
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       35
_diffrn_reflns_limit_h_min       -35
_diffrn_reflns_limit_k_max       35
_diffrn_reflns_limit_k_min       -35
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            26187
_diffrn_reflns_point_group_measured_fraction_full 0.884
_diffrn_reflns_point_group_measured_fraction_max 0.854
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.466
_diffrn_reflns_theta_min         2.599
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    2.015
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.72948
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.46 (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            white
_exptl_crystal_colour_primary    white
_exptl_crystal_density_diffrn    1.404
_exptl_crystal_description       needle
_exptl_crystal_F_000             2724
_exptl_crystal_preparation       'Solvent Exchanged in DCM'
_exptl_crystal_size_max          0.304
_exptl_crystal_size_mid          0.031
_exptl_crystal_size_min          0.029
_refine_diff_density_max         2.315
_refine_diff_density_min         -0.732
_refine_diff_density_rms         0.213
_refine_ls_abs_structure_details
;
 Flack x determined using 1023 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.027(16)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.076
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     134
_refine_ls_number_reflns         2813
_refine_ls_number_restraints     20
_refine_ls_restrained_S_all      1.073
_refine_ls_R_factor_all          0.0741
_refine_ls_R_factor_gt           0.0726
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1580P)²+60.5114P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2109
_refine_ls_wR_factor_ref         0.2127
_reflns_Friedel_coverage         0.700
_reflns_Friedel_fraction_full    0.768
_reflns_Friedel_fraction_max     0.707
_reflns_number_gt                2714
_reflns_number_total             2813
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ZnGlyPyr_DCM_100K.cif
_cod_data_source_block           ZnGlyPyr_DCM_100K
_cod_original_cell_volume        6469.4(3)
_cod_original_sg_symbol_H-M      'R 3 c'
_cod_database_code               4135199
_shelx_shelxl_version_number     2014/7
_chemical_oxdiff_formula         'Zn C6 H8 N3 O5'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_reflns_odcompleteness_completeness 99.83
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     27.41
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups, All N(H) groups
2. Rigid bond restraints
 N2, C1
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
3. Uiso/Uaniso restraints and constraints
N1 \\sim N2 \\sim C2 \\sim C3 \\sim C1: within 2A with sigma of 0.02 and sigma
for terminal atoms of 0.04
Uanis(C6) = Uanis(O2) = Uanis(O1)
4. Others
 Sof(Cl1)=Sof(Cl2)=Sof(C7)=Sof(H7A)=Sof(H7B)=FVAR(1)
5.a Secondary CH2 refined with riding coordinates:
 C5(H5A,H5B), C7(H7A,H7B)
5.b Aromatic/amide H refined with riding coordinates:
 N3(H3), C2(H2), C1(H1)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- Detector area scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.469
_oxdiff_exptl_absorpt_empirical_full_min 0.770
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x+y, y, z+1/2'
'x, x-y, z+1/2'
'-y, -x, z+1/2'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+5/6'
'x+2/3, x-y+1/3, z+5/6'
'-y+2/3, -x+1/3, z+5/6'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+7/6'
'x+1/3, x-y+2/3, z+7/6'
'-y+1/3, -x+2/3, z+7/6'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Zn1 Zn -0.69266(5) -0.68590(4) -0.13331(12) 0.0196(3) Uani 1 1 d . . . . .
Cl1 Cl -0.9201(2) -0.7407(2) -0.1341(7) 0.071(2) Uani 0.842(15) 1 d . . P . .
O2 O -0.7123(3) -0.6253(3) -0.1530(7) 0.0222(9) Uani 1 1 d . . . . .
N1 N -0.7167(4) -0.7372(4) -0.2849(8) 0.0202(16) Uani 1 1 d . U . . .
O1 O -0.7459(3) -0.7349(3) 0.0052(7) 0.0222(9) Uani 1 1 d . . . . .
Cl2 Cl -0.8320(3) -0.7124(3) -0.3279(8) 0.089(3) Uani 0.842(15) 1 d . . P . .
C5 C -0.6947(4) -0.5346(4) -0.2246(11) 0.0239(19) Uani 1 1 d . . . . .
H5A H -0.6690 -0.5096 -0.1572 0.029 Uiso 1 1 calc R . . . .
H5B H -0.6843 -0.5139 -0.3075 0.029 Uiso 1 1 calc R . . . .
N3 N -0.7513(4) -0.5491(4) -0.1914(8) 0.0204(16) Uani 1 1 d . . . . .
H3 H -0.7600 -0.5490 -0.1099 0.024 Uiso 1 1 calc R . . . .
N2 N -0.6120(4) -0.6494(4) -0.0798(9) 0.0239(18) Uani 1 1 d . U . . .
C2 C -0.7433(4) -0.7949(4) -0.2800(10) 0.0205(18) Uani 1 1 d . U . . .
H2 H -0.7559 -0.8168 -0.2037 0.025 Uiso 1 1 calc R . . . .
C3 C -0.7486(4) -0.8160(4) -0.4073(10) 0.0215(19) Uani 1 1 d . U . . .
C1 C -0.5651(5) -0.6201(4) -0.1516(10) 0.026(2) Uani 1 1 d . U . . .
H1 H -0.5647 -0.6145 -0.2422 0.031 Uiso 1 1 calc R . . . .
C6 C -0.6877(4) -0.5872(4) -0.2376(10) 0.0222(9) Uani 1 1 d . . . . .
C4 C -0.7914(4) -0.5630(5) -0.2848(10) 0.023(2) Uani 1 1 d . . . . .
C7 C -0.8475(9) -0.7176(11) -0.158(3) 0.087(9) Uani 0.842(15) 1 d . . P . .
H7A H -0.8383 -0.7444 -0.1167 0.104 Uiso 0.842(15) 1 calc R . P . .
H7B H -0.8245 -0.6808 -0.1161 0.104 Uiso 0.842(15) 1 calc R . P . .
O3 O -0.7796(4) -0.5590(5) -0.4027(8) 0.038(2) Uani 1 1 d . . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Zn1 O1 102.8(3) . . ?
N1 Zn1 O2 112.4(3) . . ?
N1 Zn1 O1 102.0(3) . . ?
N1 Zn1 N2 117.8(4) . . ?
N2 Zn1 O2 107.6(3) . . ?
N2 Zn1 O1 113.4(3) . . ?
C6 O2 Zn1 120.4(7) . . ?
N2 N1 Zn1 125.8(7) 15_434 . ?
N2 N1 C2 107.7(8) 15_434 . ?
C2 N1 Zn1 126.1(7) . . ?
C6 O1 Zn1 136.7(7) 8_345 . ?
N3 C5 C6 112.4(8) . . ?
C4 N3 C5 121.4(9) . . ?
N1 N2 Zn1 122.1(7) 8_345 . ?
C1 N2 Zn1 129.8(8) . . ?
C1 N2 N1 107.9(9) . 8_345 ?
N1 C2 C3 109.1(9) . . ?
C2 C3 C4 129.2(9) . 12_334 ?
C1 C3 C2 104.2(9) 15_434 . ?
C1 C3 C4 126.1(9) 15_434 12_334 ?
N2 C1 C3 111.0(9) . 8_345 ?
O2 C6 O1 125.2(9) . 15_434 ?
O2 C6 C5 116.7(9) . . ?
O1 C6 C5 118.1(8) 15_434 . ?
N3 C4 C3 117.7(9) . 18_334 ?
O3 C4 N3 121.4(10) . . ?
O3 C4 C3 120.8(10) . 18_334 ?
Cl1 C7 Cl2 109.9(15) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zn1 O2 1.976(7) . ?
Zn1 N1 1.953(8) . ?
Zn1 O1 1.977(7) . ?
Zn1 N2 1.975(9) . ?
Cl1 C7 1.76(2) . ?
O2 C6 1.249(12) . ?
N1 N2 1.359(11) 15_434 ?
N1 C2 1.360(13) . ?
O1 C6 1.267(12) 8_345 ?
Cl2 C7 1.77(3) . ?
C5 N3 1.421(13) . ?
C5 C6 1.539(14) . ?
N3 C4 1.346(13) . ?
N2 N1 1.358(11) 8_345 ?
N2 C1 1.331(14) . ?
C2 C3 1.389(14) . ?
C3 C1 1.374(15) 15_434 ?
C3 C4 1.480(14) 12_334 ?
C1 C3 1.374(15) 8_345 ?
C6 O1 1.267(12) 15_434 ?
C4 C3 1.480(14) 18_334 ?
C4 O3 1.227(13) . ?
